Biocomposites for Adsorptive Wastewater TreatmentView this Special Issue
Recent Review of Titania-Clay-Based Composites Emerging as Advanced Adsorbents and Photocatalysts for Degradation of Dyes over the Last Decade
Textile industry being one of the most flourishing industries keeps growing and developing every year, and the consequences are not very pleasant. Even though its contribution towards economy of a country is indisputable, there are many pros and cons associated with it that should not be brushed aside, one of them being textile dye waste which is also growing at alarming rate. Many techniques have been designed to deal with this environmental crisis including adsorption and photodegradation of dye waste by various substances, both natural and synthetic. TiO2 and clay both have gained immense popularity in this area. Over the last decade, many successful attempts have been made to design TiO2-clay-based composites to combine and make the most of their individual capabilities to degrade textile dye waste. While clay is an effective adsorbent, inexpensive, innocuous, and a great ion exchanger, TiO2 provides supplementary active sites and free radicals and speeds up the degradation rate of dyes. This review summarizes various features of TiO2-clay-based composites including their surface characteristics, their role as dye adsorbents and photocatalysts, challenges in their implementation, and modifications to overcome these challenges made over the last decade.
Color is defined as optical interpretation originating from the brain when visible light stimulates the human eye . The discovery of earliest dye (aniline purple) dates back to the 1860s by W.H. Perkin who laid the foundation for worldwide production of dyes for commercial purposes . Initially, the world relied on Europe for manufacture and supply of dyes, but currently, South Asia has overtaken it . Gross production of dyes is expected to be 1,000,000 tons per year . These dyes are used in the fabrics, processing of leather, publication, lithography, medicinal, and beauty sectors. Some of them are also used as coloring agents for food items . This universal reliance of industrial sectors on dyes means that a bulk amount of dye effluents are being produced and dumped over by every industry all over the world and most of it is discarded into water bodies. It has been reported that 200 BL dye effluents are being discharged in water per year [6, 7]. Some examples of commonly used dyes have been listed in Table 1. Most of them are used extensively in textile and chemical industries, like brilliant green, Congo red, methylene blue, and indigo carmine. Many dyes are stable towards degradation and it is hard to decompose them, resulting effluents using ordinary methods of wastewater treatment . These dye effluents have been reported to cause cancer, allergies, and skin diseases; therefore, their proper treatment is inevitable . Figure 1 gives a brief description of procedures involved in textile waste water treatment.
It involves various physical and chemical treatment methodologies, like coagulation, ozonation, bioremediation, filtration, photochemical degradation, and electrolysis, either individually or in combination to produce clean water. That water in turn is used for secondary purposes, like watering plants, washing, steam generators, and leaching. Some types of water treatments even produce pure water that can be used for drinking, like in Sri Lanka and Malaysia, and desalination and ion exchange processes are used to convert sewage and sea water into drinkable one.
1.1. Toxicological Profile of Dyes
Dye effluents mainly pollute environment in the form of water pollutants which are released into water system without treatment. It causes a significant drop in oxygen concentration of water as sulfur hydrides screen the light from entering the aqueous streams which leads to a deleterious effects on aquatic environment. Half of these dye effluents may have chlorine in their composition which is a mutagen and cancerous in nature. Some dyes may also consist of metal ions, like Hg, Cd, As, Cr, and Pb which cannot be decomposed biologically, so they have the tendency to accumulate in our immune system, causing deterioration and inducing different maladies. Unprocessed or partly decomposed dye pollutants are destructive for both aquatic and human life . Table 2 enlists chief human maladies caused by dye pollutants.
1.2. Degradation Methods of Dye Effluents
Since the time, the pathological effects of dye effluents have been analyzed, and researchers have been working on various effective techniques for their decomposition and removal from wastewater. Some of these techniques have been showcased in Figure 2. They are widely explored all over the world by different researchers. Most of them were employed on industrial level for wastewater treatment or for converting sea water into pure water.
Amongst all these methods, adsorption has emerged as an exceptionally effective and facile method for the removal of dye effluents (Table 3) . Adsorption is a physical phenomenon of separation of any element between two surfaces, e.g., liquid/solid. It can be carried out by physical or chemical means. One of its main features is regeneration of adsorbent. The adsorption potential of a substance depends on its surface area, resistance to abrasion, pore diameter and structure, etc. . It is quite simplistic and economically favorable and involves swift recollection and reusability of adsorbent without needing to deal with sludge or unsafe side products. However, the success of adsorption procedure depends on performance of adsorbents which should be comprehensive in its actions. Sometimes an adsorbent may observe a very high adsorption potential but lack other important features. For instance, activated carbon is a commonly used adsorbent having a high SSA (specific surface area), void fraction, and adsorption efficiency, but its heavy price and complexed isolation post sorption has limited its usage. Therefore, scientists have been engrossed in designing such adsorbents which are not only effective in action but also strong, durable, renewable, cost-efficient, and eco-friendly .
1.2.2. Adsorption Kinetics
The adsorption potential of an adsorbent is represented graphically using different models such as Freundlich and Langmuir . These graphs are based on concentration of adsorbate adsorbed by adsorbent at constant parameters (temperature and pressure) .
The Langmuir model (Equation (1)) perfectly represents a single-layer adsorption unit. It is based on the assumption that dye particles when adsorbed on adsorbent arrange themselves in a single layer, all the adsorbed particles having equal amount of . It also suggests that single-dye particle binds per active site. Moreover, this theory overlooks the interactivity between individual dye particles . where : Adsorption potential at equilibrium (mgg-1), : Max adsorption potential (mgg-1), : Conc. of adsorbed dyes at equilibrium (mgL-1), : Equilibrium constant of adsorption (Lmg-1).
Contrary to the Langmuir model, the Freundlich model (Equation (2)) represents an adsorption theory where dye particles are adsorbed and arrange in more than one layer and this arrangement is nonlinear . Mostly, the Freundlich model is used where more refined adsorbents with enlarged surfaces and better pore morphology are being studied for adsorption or to describe the adsorption of extremely reactive organic dyes . Although these equations are perfectly applicable at low pressure, the values become more uncertain at high pressure . where : Adsorption potential at equilibrium (mgg-1), : Adsorption potential (mmolg-1), Ce: Conc. of adsorbed dyes at equilibrium (mgL-1), : Constant of adsorption strength.
Both these models have been used to study kinetics of adsorption for various adsorbents [39–41]. Some other models that have also been proved quite successful are Temkin  and Henry’s . Koyuncu and Okur used all these four models to study adsorption potential of C2M1 for AV 90 dye where the Freundlich model proved to be superior than others having highest correlation factor () , while Kulasooriya et al. investigated adsorption potential of brick clays for SBE dye where the Langmuir model showed better results, max adsorption potential being 1667 mg kg-1 .
1.2.3. Parameters for Effective Adsorption of Dyes
The process of adsorption is dependent on parameters like pH, heat, and quantity of adsorbent. Different parameters have different impact on different adsorbents. Some conditions could be more ideal for one adsorbent but not for others. Therefore, optimum parameters are decided for every adsorbent on hit and trial basis.
(1) Temperature. Adsorption is either exothermic or endothermic so temperature is a major parameter here. In an endothermic procedure, the value of rises at higher temperature due to enhanced motion of the dye particles and increased active sites of adsorbents . However in some cases, value of falls at higher temperature as motion of dye particles slows down and adsorption is exothermic .
(2) Quantity of Adsorbent. Usually, the greater the quantity of adsorbents, the greater the number of active sites available and hence the higher is adsorption potential . However, financially feasible adsorbents are those that show higher potential with minimum quantity .
(3) pH. pH is another major parameter that impacts adsorption procedure determined by pzc (point of zero charge). pH can control rate of ionization of the adsorbents. Cationic dyes show lower adsorptions at lower pH and higher adsorption at higher pH, while it is opposite for anionic dyes . Cationic dyes show greater adsorptions if pH of solution is higher than pHpzc, while it is opposite for anionic dyes .
Unlike adsorption, photocatalysis is an advanced technique which has been proved as an effective remediation for waste water treatment. This procedure does not require the usage of any strong chemical specie, so the chances of production of hazardous side products are very little. Photocatalysis is powerful enough to decompose otherwise highly stable dyes into harmless products . The fundamental principle of photocatalysis involves the contact between dye pollutants and their loading onto the photocatalyst. The dye pollutants get adsorbed on its exterior where redox reactions transpire as a result of generation of electrons from conduction band (CB) and holes from valence band (VB). The resultant products finally detach from the photocatalyst and are discarded into the aqueous media . The reaction mechanism can be simplified as follows:
Various studies have proved that photocatalysis is a highly efficient and result-oriented technique for degradation of dyes.
Photocatalysis can be carried out via batch as well as continuous process as shown in Figure 3.
This review mainly focuses on progress made on clay-based TiO2 composites over the period of past decade. It summarizes the data on the synthesis and implementation of clay-TiO2 composites for treatment of industrial waste water, both as adsorbent or as a photocatalyst. A literature review based on selective experimental approaches was made which highlights the advantage of degradation of dyes by clay-based TiO2 composites.
2. TiO2 as Adsorbent and Photocatalyst and Its Limitations
TiO2 is an excellent adsorbent based on its abundance, ease of excitability, modifiable physical properties, and a very fitting PCZ of 6–6.8, which enables it to adsorb dye particles . TiO2 is also a widely used photocatalyst owing to its degradation potential . Photocatalysis obviously cannot be carried out without adsorption of dyes onto TiO2. This adsorption brings out the interaction between the dye particles and photogenerated species, which kick starts photocatalysis . Thus, the photocatalytic activity of TiO2 is also determined by its adsorption potential. Adsorption is a surface phenomenon which is dependent on form, area, and structural regularity of TiO2 crystals .
TiO2 is highly stable both chemically and physically and mild and inexpensive which make it a perfect photocatalyst . TiO2 exhibits polymorphism and its 3 mineral forms are anatase, brookite, and rutile [59, 60]. Anatase and rutile are reported to have greater photocatalytic activity. Anatase is a better photocatalyst owing to its indirect band gap that gives a greater life span to electron-hole pair, while rutile produces electron-hole pair of a shorter life span based on its direct band gap . CB and VB of TiO2 have a gap of 3.2 eV (anatase) and 3.0 eV (rutile) . Thus, anatase has a of 387.5 and rutile has 400 nm in UV region . TiO2 on photoexcitation produces a number of electrons and holes in CB and VB simultaneously. These charged species further create bunch of free radicals which forms the core of photodegradation mechanism . The mechanism is briefly explained through Figure 4 graphically.
2.1. Drawbacks and Challenges
However, TiO2 has few drawbacks  that can make it less effective and various methods have been adopted to overcome them. (1)A very large band gap of anatase limits its ability to adsorb light in UV region only, so it cannot make proper use of spectrum. To overcome this problem, TiO2 has been modified by induction of metallic [66, 67] and certain nonmetallic [68, 69] compounds which shrink the band gap as shown in Figure 5(2)Lesser attraction for organic dyes and lesser volume of pores per surface area reduce its adsorption potential. So adsorption capacity of organic dyes is improved by layering its surface with carbon-based organic compounds [70, 71](3)Irregular distribution of TiO2 particles and agglomeration of its NPs can block the active sites and hinder the interaction with incoming light. To avoid this, TiO2 is immobilized with different supports which break off clustering of its particles and blockage of light [72, 73](4)It often ends up making a slurry in liquid media and its regeneration gets difficult which makes its use less cost-effective. Functionalization by magnetization of TiO2 can make its recovery easier [74, 75]
2.1.1. Clay as an Adsorbent and an Effective Support for Titania
Clay is a mineral naturally found on earth crust. Its chief composition is finely grounded substances (mostly sheet silicates) that impart a unique plasticity in aqueous media, while it hardens up in dry conditions . Clay composition involves uniformly grounded hydrated alumino-silicates. The structure of these alumino-silicates contains tetrahedral sheets of Si-O and octahedral sheets of Al. Clay has the potential to clean wastewater system up to 70% by adsorbing impurities . The extent to which these impurities are adsorbed onto clay depends on how strongly they interact with natural clay and mineral oxides on its surface [78–82]. The adsorption procedure is regulated by a few factors such as nature of ions (cationic or anionic), number of ions, pH, temperature, and nature of dye being treated [83, 84].
Clays have emerged as popular supports for TiO2 for dye degradation. (1)Pure TiO2 has lower photocatalytic potential than clay-based TiO2 composite. Clay imparts TiO2 a larger surface area, increases the number of active sites, and hence improves its adsorption potential (2)Cations are present in between the layers of clay structure which captures the electrons. Thus, the holes in VB of TiO2 are free and available for oxidization. This reduces the overall rate of charge recombination in TiO2-clay composites and increases its photocatalytic potential (3)Regeneration and recovery of TiO2-clay composites are easier due to the presence of charged species on clay which make the composite separable from aqueous media and the reaction becomes more feasible economically
2.2. Preparation of TiO2-Clay Composites
TiO2-clay-based composites can be synthesized using various techniques as shown in Figure 6. They are reported by various researchers from all over the world with good yields and various applications.
2.2.1. Adsorption of Dyes via TiO2-Clay Composites
TiO2/stishovite clay composite was simply prepared by mixing stishovite and TiO2 and stirring with alcohol for 5-6 hours, precipitating overnight, and vacuum drying. The resultant composite was used for adsorption of MV dye. 88% of dye was adsorbed. The adsorption data shows that adsorbent’s surface was covered by a single layer. Adsorption process was endothermic and it observed pseudo 2nd order. However, the recovery rate of adsorbent was not up to the mark .
Likewise, a TiO2-bentonite composite was prepared by mixing TiO2 with clay and double distilled H2O followed by stirring and drying, and the resulting composite was used for degradation of RhB via batch process and results were studied using the Langmuir isotherm. TiO2-bentonite adsorbent removed up to 98.9% RhB which was higher than natural clay adsorbent .
TiO2 has the ability to make composites with a variety of clays. TiO2-rectorite composite was synthesized by mixing titanium butoxide/HCl suspension with rectorite/dd H2O suspension followed by stirring, drying, centrifugation, washing, and finally drying. Then, it was magnetized with iron oxide and used for adsorption of MB dye showing max adsorption potential of 169.20 mgg-1. Iron oxide was reported to increase the number of active sites by rupturing the sheets of TiO2-rectorite composite and created large cavities which adsorbed greater number of MB molecules. Magnetization also made desorption easier .
The degradation potential of TiO2-clay composites can be enhanced by incorporation of metal oxides. TiO2-WO3-bentonite composites were synthesized through hydrothermal method by adding a mixture of Na+-bentonite and sodium tungstate dihydrate mixture to titanium tetrachloride with constant mixing in a cold bath followed by treatment with ultrasound radiations for ½ hr. This mixture was heated in an autoclave with H2O at 443.15 K for 10 h. The resultant composite was separated through filtration and washed and dried at 25°C. This composite was used for adsorption studies of MB dye. WO3 has been reported to escalate TiO2’s sensitivity for gaseous species as well as improves its acidic strength and increases its affinity for dye contaminants. The unique pretreatment of bentonite with ultrasound radiations allowed a thorough disruptor of Na+-bentonite matrix and uniform insertion and intercalation of TiO2-WO3 particles in between its layers. The adsorbent exhibited excellent adsorbent potential, a smooth desorption, and an easy recovery. Moreover, the adsorption potential of pretreated adsorbent increased by 50% possibly due to increase in number of active sites by ultrasound irradiation .
Mixing of TiO2 with clay and organic material like graphene imparts its tremendous adsorption properties. TiO2-palygorskite-graphene composite was prepared via hydrothermal method, while CTAB was used as a surface active agent and adsorption of MB was studied. The studies suggest that graphene having layers of sp2 hybridized C is bestowed with a huge surface area, greater affinity for H2O, and uniform distribution which makes it an ideal support. Likewise, palygorskite has exceptional adsorption potential owing to its enormous surface area and heat resistance. C=O groups on the surface of adsorbent provided the active sites where MB molecules were seem to be bound by H-bonds (on OH groups). The adsorbent showed commendable adsorption even after 5 recovery cycles. The max adsorption potential was 134.59 mgg-1 .
Clay composites of TiO2 can be further improved by microwave treatment. TiO2-bentonite composite was synthesized via impregnation where bentonite was added to a water suspension of TiO2 followed by heating and stirring. The thoroughly mixed solution was subjected to microwave irradiation; the product was removed and desiccated. It was further used to study adsorption behavior using RhB and MB dyes using the Langmuir equation. Structural analysis shows that the integration of TiO2 particles onto bentonite via impregnation enhanced its adsorption potential, and OH● on TiO2 act as potential active sites and amplify the adsorption process .
A TiO2-Rouge clay composite was synthesized via hydrothermal synthesis. Carefully refined and pretreated clay (with NaOH) was purified and desiccated and stored for 12 hours. Equal weight of functionalized clay and TiO2 were mixed in the presence of NaOH at 373.15 K and 5 atm. The adsorbent was used for adsorption of MB dye; it was reported to remove 91.19% dye. Morphological analysis indicates that the clay undergoes structural rearrangement post combination with TiO2 and adsorbent shows a comparatively uneven and granulated surface with multiple active sites which escalates adsorption rate .
Lately, halloysite nanotubes (financially feasible clays) have enticed deep interest owing to their hollow tube-like structure, enlarged surface area, and distinctive surface features. A TiO2-halloysite composite was doped with Fe using hydrothermal procedure and used for adsorption of RhB and MB dyes. The multilayer tubes have anionic Si–OH on the exterior side and cationic Al–OH on the interior side which attract impurities of different nature via electrostatic interactions. Moreover, they are harmless, inexpensive, easily accessible, and nonhazardous. TiO2-Fe composites were seen to stick to the exterior of the tubes which increased their dispersion in aqueous phase, and the greater the dispersion, greater the contact with dye contaminants present in water and hence the higher the adsorption .
Table 4 gives a brief summary of synthesis methodologies and application of some of TiO2-clay-based composites in degradation of dyes via adsorption.
2.2.2. Photocatalysis of Dyes via TiO2-Clay Composites
Mixing different phases of TiO2 with clay gives amazing results in photocatalysis. A novel TiO2-kaolinite photocatalyst was prepared using various phases of TiO2 which was used for photocatalytic degradation of ARG dye. According to XRD data, the photocatalyst seemed to be composed of mixtures of 3 different phases of TiO2, i.e., anatase, rutile, and brookite, in different combinations. The anatase/brookite combination was reported to have highest photoactivity. Both of them were stimulated by UV light which leads to photogeneration of free electrons in anatase. Anatase has a highly negative CB so these electrons diffuse to brookite. These electrons undergo a series of reactions and produce •OH which oxidizes dye particles. Likewise, photoactivated holes in brookite diffuse to anatase due to its high VB potential and interact with dye particles. Thus, the mixing of different phases and resulting heterojunction between them can improve TiO2’s photocatalysis .
The amount of clay used in the composite plays an important role in its potential to remove impurities. A TiO2/clinoptilolite photocatalyst was prepared via sol-gel method in different ratios and used for degradation of CN and MV-2B dye. The charge on the surface was dependent on clay’s ratio which is an important factor in determining the affinity of charged dye particles towards the photocatalyst. 90/10 turned out to be the best ratio; the lower the clay ratio, the higher was the surface area and photocatalysis. The lower ratio of clay also prevented accumulation of TiO2 in aqueous phase and improved its recovery .
Rapsomanikis et al. prepared TiO2-halloysite clay composites using sol-gel method for photocatalysis of BB41. The unique feature of this photocatalyst was that its surface was modified with Ag particles by treating composite’s films with 1.0 mM AgNO3 sol for 10-20 minutes followed by rinsing with double distilled H2O and drying by N2 gas. Later, the Ag ions were reduced to Ag0 by UV irradiation of films. These Ag particles were reported to improve TiO2’s efficiency to separate charge carrying species which led to an enhanced photocatalytic activity .
Even though TiO2-clay photocatalyst show a remarkable potential to degrade dyes and are economically feasible, some of them (e.g., TiO2-palygorskite) have limited applications as they can only be stimulated by ultraviolet light owing to their large . Various experiments have been carried out to make them responsive to visible light, some of which include hybridization and doping with other metals especially transition metals. The plasmonic effects of Ag nanoparticles enable it to improve the visible light sensitivity of TiO2-clay photocatalysts and expand their area of usage. A TiO2-Palgorskite composite was doped with Ag-AgCl particles through deposition-photoreduction method and used for photocatalytic degradation of RhB. Due to the surface plasmonic effect, Ag nanoparticles improved the photoactivity of the catalyst under visible light .
The sensitivity of TiO2 towards light spectrum can also be broadened by merging it with other metal oxides like Fe2O3 which are highly photoactive under visible light due to Fenton mechanism. Therefore, its fusion with TiO2 imparts an exceptional photoactivity under natural day light, which is a mixture of ultraviolet (5%) and visible (40%) and IR light (55%). One such photocatalyst was prepared through sol-gel procedure where bentonite-supported TiO2 was doped with Fe2O3 and used for photocatalysis of MB. The dye was completely degraded in 2 hours. Fe2O3 not only improved the photoactivity by absorption of light in visible region, but its magnetic nature also helped to retrieve and reuse the photocatalyst making it economically favorable .
Another such attempt to exploit visible light for photodegradation by TiO2-clay composites was made by depositing g-C3N4 onto TiO2-bentonite via wet impregnation. For this purpose, TiO2-bentonite composite was mixed with highly concentrated slurry of g-C3N4, sonicated for 120 minutes, stirred overnight, and dried at 333.15 K. Samples of such composites with varying weight of g-C3N4 were prepared. These composites were applied for photodegradation of RBR dye. 90% of the dye was degraded within 1.6 hour under visible light. This brilliant outcome was ascribed to strong interaction between clay and g-C3N4 leading to enhanced dispersity, increased number of active sites, and their uniform distribution and better optical activity. Another reason was rate of charge recombination declined due to electron transfer from g-C3N4 to TiO2 and photoinduction under visible light. The photocatalyst was reusable for 5 successive cycles .
Incorporation of nonmetallic additives like urea into TiO2-clay composites can be quite favorable. Urea is reported to promote formation of anatase phase and contributes to porosity of the TiO2-clay composite that adds to photocatalytic potential. Urea addition can also lead to shrinkage of the band gap of the TiO2-clay composite from 3.35 to 2.92 eV and makes it visible light activated. It is reported to enhance the degradation rate of dyes by 2.3 times under visible lights. Moreover, it is inexpensive and easily available which makes it even a better additive .
Photocatalytic degradation coupled with ultrasound treatment has been proved a very effective technique to enhance photoactivity of TiO2-clay composites. During photocatalysis, the efficiency of photocatalyst is reduced over the time due to blockage of active sites and hindrance of UV light. Ultrasonic treatment solves this problem by acting as an irradiation sources and activates TiO2 to carry out sono-catalysis in the absence of UV light. Ultrasound waves also induce turbulence in the liquid phase which results in particle sizing and deagglomeration and hence increase number of active sites available. Moreover, treatment of these titania-clay composites with ultrasound waves leads to formation of supplementary OH• radicals. All these factors are reported to escalate photoactivity of titania-clay composites and speed up the removal rate of dye .
Table 5 gives a brief summary of synthesis methodologies and application of some of titania-clay-based composites in degradation of dyes via photocatalytic degradation.
It is evident from Tables 4 and 5 comparisons that sol-gel and coprecipitation methods are more used for synthesizing titania-clay composites as compared to other methodologies.
(i)TiO2 as both photocatalyst and adsorbent is extensively and effectively used for treatment of textile waste water(ii)The factors that limit TiO2’s efficacy of dye degradation can be overcome by using different supports like clays, silica, etc.(iii)Clays like rectorite, bentonite, montmorillonite, attapulgite, kaolinite, and halloysite are most commonly used as supports for TiO2 using various techniques(iv)Clay as a support provides TiO2 with a high surfaces area, porosity, improved morphology, more active sites, and better adsorption of dyes(v)Loading of TiO2 on clays helps preventing the aggregation of TiO2 and its loss to environment(vi)The efficacy of these TiO2-clay composites can be enhanced by further addition of various metallic and nonmetallic substances, ultrasonic irradiation, and experimenting with different phases and particle size of TiO2(vii)These TiO2-clay composites are energy-efficient, nonhazardous, and economically feasible(viii)The study on TiO2-clay-based composites and their modifications for treatment of textile waste water is a rapidly growing field of science
All data related to this work is presented in results section along with references.
Conflicts of Interest
The authors declare that they have no conflicts of interest regarding the publications of this review.
Authors are thankful to home institute library for this review data collection.
R. Christie, “Colour Chemistry,” The Royal Society of Chemistry, RSC Paperbacks, pp. 1–11, 2001.View at: Google Scholar
L. Pereira and M. Alves, “Dyes—environmental impact and remediation,” Environmental Protection Strategies for Sustainable Development, Springer, pp. 111–162, 2012.View at: Google Scholar
A. E. Ghaly, R. Ananthashankar, M. V. Alhattab, and V. V. Ramakrishnan, “Production, characterization and treatment of textile effluents: a critical review,” Journal of Chemical Engineering & Process Technology, vol. 5, no. 1, pp. 1–19, 2014.View at: Google Scholar
S. Arora, “Textile dyes: it's impact on environment and its treatment,” Journal of Bioremediation & Biodegredation, vol. 5, no. 3, p. 1, 2014.View at: Publisher Site | Google Scholar
P. Bamfield, Chromic phenomena: technological applications of colour chemistry, Royal Society of Chemistry, 2010.
R. Kant, “Textile Dyeing Industry an Environmental Hazard,” Natural Science, vol. 4, no. 1, pp. 22–26, 2012.View at: Publisher Site | Google Scholar
T. Puzyn and A. Mostrag, Organic pollutants ten years after the Stockholm convention: environmental and analytical update, BoD–Books on Demand, 2012.
H. Ali, “Biodegradation of synthetic dyes—a review,” Water, Air, & Soil Pollution, vol. 213, no. 1-4, pp. 251–273, 2010.View at: Publisher Site | Google Scholar
F. D. Chequer, G. R. De Oliveira, E. A. Ferraz, J. C. Cardoso, M. B. Zanoni, and D. P. De Oliveira, “Textile dyes: dyeing process and environmental impact,” Eco-Friendly Textile Dyeing and Finishing, vol. 6, pp. 151–176, 2013.View at: Google Scholar
S. Gita, A. Hussan, and T. Choudhury, “Impact of textile dyes waste on aquatic environments and its treatment,” Environment and Ecology, vol. 35, no. 3C, pp. 2349–2353, 2017.View at: Google Scholar
F. M. D. Chequer, J. P. F. Angeli, E. R. A. Ferraz et al., “The azo dyes disperse red 1 and disperse orange 1 increase the micronuclei frequencies in human lymphocytes and in HepG2 cells,” Mutation Research, Genetic Toxicology and Environmental Mutagenesis, vol. 676, no. 1-2, pp. 83–86, 2009.View at: Publisher Site | Google Scholar
S. Mani and R. N. Bharagava, “Exposure to crystal violet, its toxic, genotoxic and carcinogenic effects on environment and its degradation and detoxification for environmental safety,” Reviews of Environmental Contamination and Toxicology Volume, vol. 237, pp. 71–104, 2016.View at: Publisher Site | Google Scholar
M. Tsuboy, J. P. F. Angeli, M. S. Mantovani, S. Knasmüller, G. A. Umbuzeiro, and L. R. Ribeiro, “Genotoxic, mutagenic and cytotoxic effects of the commercial dye CI disperse blue 291 in the human hepatic cell line HepG2,” Toxicology In Vitro, vol. 21, no. 8, pp. 1650–1655, 2007.View at: Publisher Site | Google Scholar
F. Ding, L. Zhang, J. X. Diao, X. N. Li, L. Ma, and Y. Sun, “Human serum albumin stability and toxicity of anthraquinone dye alizarin complexone: an albumin-dye model,” Ecotoxicology and Environmental Safety, vol. 79, pp. 238–246, 2012.View at: Publisher Site | Google Scholar
S. Chawla, H. Uppal, M. Yadav, N. Bahadur, and N. Singh, “Zinc peroxide nanomaterial as an adsorbent for removal of Congo red dye from waste water,” Ecotoxicology and Environmental Safety, vol. 135, pp. 68–74, 2017.View at: Publisher Site | Google Scholar
H. Yagi, A. M. el Hendi, A. Diab, and A. A. Elshikh, “Paraphenylenediamine induced optic atrophy following hair dye poisoning,” Human & Experimental Toxicology, vol. 15, no. 8, pp. 617-618, 1996.View at: Publisher Site | Google Scholar
E. Helaskoski, H. Suojalehto, H. Virtanen et al., “Occupational asthma, rhinitis, and contact urticaria caused by oxidative hair dyes in hairdressers,” Annals of Allergy, Asthma & Immunology, vol. 112, no. 1, pp. 46–52, 2014.View at: Publisher Site | Google Scholar
T. Kaji, T. Kawashima, M. Sakamoto, Y. Kurashige, and F. Koizumi, “Inhibitory effect of rhodamine B on the proliferation of human lip fibroblasts in culture,” Toxicology, vol. 68, no. 1, pp. 11–20, 1991.View at: Publisher Site | Google Scholar
D. Ghosh, P. S. Singha, S. B. Firdaus, and S. Ghosh, “Metanil yellow: the toxic food colorant,” Asian Pacific Journal of Health Sciences, vol. 4, no. 4, pp. 65-66, 2017.View at: Publisher Site | Google Scholar
H. Pan, J. Feng, G. X. He, C. E. Cerniglia, and H. Chen, “Evaluation of impact of exposure of Sudan azo dyes and their metabolites on human intestinal bacteria,” Anaerobe, vol. 18, no. 4, pp. 445–453, 2012.View at: Publisher Site | Google Scholar
D. Pelclová, P. Rössner, and J. Picková, “Chromosome aberrations in rotogravure printing plant workers,” Mutation Research Letters, vol. 245, no. 4, pp. 299–303, 1990.View at: Publisher Site | Google Scholar
E. Kus and H. E. Eroglu, “Genotoxic and cytotoxic effects of sunset yellow and brilliant blue, colorant food additives, on human blood lymphocytes,” Pakistan Journal of Pharmaceutical Sciences, vol. 28, no. 1, 2015.View at: Google Scholar
K. S. Rowe and K. J. Rowe, “Synthetic food coloring and behavior: a dose response effect in a double-blind, placebo-controlled, repeated-measures study,” The Journal of Pediatrics, vol. 125, no. 5, pp. 691–698, 1994.View at: Publisher Site | Google Scholar
N. Toxicology, Carcinogenesis Studies of Naphthalene (CAS No 91-20-3) in B6C3F1 Mice (Inhalation Studies), US Department of Health and Human Services. Public Health Service, National Institutes of Health, Research Triangle Park, NC, 1992.
E. L. Opie, “The pathogenesis of tumors of the liver produced by butter yellow,” The Journal of Experimental Medicine, vol. 80, no. 3, pp. 231–246, 1944.View at: Publisher Site | Google Scholar
K.-T. Chung, “Azo dyes and human health: a review,” Journal of Environmental Science and Health, Part C, vol. 34, no. 4, pp. 233–261, 2016.View at: Publisher Site | Google Scholar
H. Sun, Y. Liu, M. Li, S. Han, X. Yang, and R. Liu, “Toxic effects of chrysoidine on human serum albumin: isothermal titration calorimetry and spectroscopic investigations,” Luminescence, vol. 31, no. 2, pp. 335–340, 2016.View at: Publisher Site | Google Scholar
C. Vidya, C. Manjunatha, M. Sudeep, S. Ashoka, and M. A. Lourdu Antony Raj, “Photo-assisted mineralisation of titan yellow dye using ZnO nanorods synthesised via environmental benign route,” SN Applied Sciences, vol. 2, no. 4, pp. 1–15, 2020.View at: Publisher Site | Google Scholar
C. D. Raman and S. Kanmani, “Textile dye degradation using nano zero valent iron: a review,” Journal of Environmental Management, vol. 177, pp. 341–355, 2016.View at: Publisher Site | Google Scholar
A. A. Siyal, M. R. Shamsuddin, A. Low, and N. E. Rabat, “A review on recent developments in the adsorption of surfactants from wastewater,” Journal of Environmental Management, vol. 254, p. 109797, 2020.View at: Publisher Site | Google Scholar
A. Azari, R. Nabizadeh, S. Nasseri, A. H. Mahvi, and A. R. Mesdaghinia, “Comprehensive systematic review and meta-analysis of dyes adsorption by carbon-based adsorbent materials: classification and analysis of last decade studies,” Chemosphere, vol. 250, p. 126238, 2020.View at: Publisher Site | Google Scholar
L. Largitte and R. Pasquier, “A review of the kinetics adsorption models and their application to the adsorption of lead by an activated carbon,” Chemical Engineering Research and Design, vol. 109, pp. 495–504, 2016.View at: Publisher Site | Google Scholar
T. H. Tran, A. H. le, T. H. Pham et al., “Adsorption isotherms and kinetic modeling of methylene blue dye onto a carbonaceous hydrochar adsorbent derived from coffee husk waste,” Science of the Total Environment, vol. 725, p. 138325, 2020.View at: Publisher Site | Google Scholar
Y. Zhou, R. Zhang, X. Gu, and J. Lu, “Adsorption of divalent heavy metal ions from aqueous solution by citric acid modified pine sawdust,” Separation Science and Technology, vol. 50, no. 2, pp. 245–252, 2015.View at: Publisher Site | Google Scholar
L. Czepirski, M. R. Balys, and E. Komorowska-Czepirska, “Some generalization of Langmuir adsorption isotherm,” Internet Journal of Chemistry, vol. 3, no. 14, pp. 1099–8292, 2000.View at: Google Scholar
J. Appel, “Freundlich's adsorption isotherm,” Surface Science, vol. 39, no. 1, pp. 237–244, 1973.View at: Publisher Site | Google Scholar
S. F. Azha, L. Sellaoui, E. H. Engku Yunus et al., “Iron-modified composite adsorbent coating for azo dye removal and its regeneration by photo-Fenton process: synthesis, characterization and adsorption mechanism interpretation,” Chemical Engineering Journal, vol. 361, pp. 31–40, 2019.View at: Publisher Site | Google Scholar
J. Wang and X. Guo, “Adsorption isotherm models: classification, physical meaning, application and solving method,” Chemosphere, vol. 258, p. 127279, 2020.View at: Publisher Site | Google Scholar
Z. Li, H. Hanafy, L. Zhang et al., “Adsorption of Congo red and methylene blue dyes on an ashitaba waste and a walnut shell-based activated carbon from aqueous solutions: experiments, characterization and physical interpretations,” Chemical Engineering Journal, vol. 388, p. 124263, 2020.View at: Publisher Site | Google Scholar
A. H. Jawad and A. S. Abdulhameed, “Mesoporous Iraqi red kaolin clay as an efficient adsorbent for methylene blue dye: adsorption kinetic, isotherm and mechanism study,” Surfaces and Interfaces, vol. 18, p. 100422, 2020.View at: Publisher Site | Google Scholar
F. Ali, N. Ali, I. Bibi et al., “Adsorption isotherm, kinetics and thermodynamic of acid blue and basic blue dyes onto activated charcoal,” Case Studies in Chemical and Environmental Engineering, vol. 2, p. 100040, 2020.View at: Publisher Site | Google Scholar
R. Jabbari and N. Ghasemi, “Investigating methylene blue dye adsorption isotherms using silver nano particles provided by aqueous extract of Tragopogon buphthalmoides,” Chemical Methodologies, vol. 5, no. 1, pp. 21–29, 2021.View at: Google Scholar
G. R. Delpiano, D. Tocco, L. Medda, E. Magner, and A. Salis, “Adsorption of malachite green and alizarin red S dyes using Fe-BTC metal organic framework as adsorbent,” International Journal of Molecular Sciences, vol. 22, no. 2, p. 788, 2021.View at: Publisher Site | Google Scholar
D. D. E. Koyuncu and M. Okur, “Removal of AV 90 dye using ordered mesoporous carbon materials prepared via nanocasting of KIT-6: adsorption isotherms, kinetics and thermodynamic analysis,” Separation and Purification Technology, vol. 257, article 117657, 2021.View at: Publisher Site | Google Scholar
T. Kulasooriya, N. Priyantha, and A. Navaratne, “Removal of textile dyes from industrial effluents using burnt brick pieces: adsorption isotherms, kinetics and desorption,” SN Applied Sciences, vol. 2, no. 11, pp. 1–11, 2020.View at: Google Scholar
M. Adel, M. A. Ahmed, and A. A. Mohamed, “A facile and rapid removal of cationic dyes using hierarchically porous reduced graphene oxide decorated with manganese ferrite,” FlatChem, vol. 26, p. 100233, 2021.View at: Publisher Site | Google Scholar
S. Chakraborty, A. Mukherjee, S. Das, N. Raju Maddela, S. Iram, and P. Das, “Study on isotherm, kinetics, and thermodynamics of adsorption of crystal violet dye by calcium oxide modified fly ash,” Environmental Engineering Research, vol. 26, no. 1, p. 26(1), 2021.View at: Publisher Site | Google Scholar
E. Altintig, A. Alsancak, H. Karaca, D. Angın, and H. Altundag, “The comparison of natural and magnetically modified zeolites as an adsorbent in methyl violet removal from aqueous solutions,” Chemical Engineering Communications, vol. 209, no. 4, pp. 555–569, 2022.View at: Publisher Site | Google Scholar
M. Hijab, P. Parthasarathy, H. R. Mackey, T. al-Ansari, and G. McKay, “Minimizing adsorbent requirements using multi-stage batch adsorption for malachite green removal using microwave date-stone activated carbons,” Chemical Engineering and Processing Process Intensification, vol. 167, p. 108318, 2021.View at: Publisher Site | Google Scholar
X. Zhao, X. Wang, and T. Lou, “Preparation of fibrous chitosan/sodium alginate composite foams for the adsorption of cationic and anionic dyes,” Journal of Hazardous Materials, vol. 403, p. 124054, 2021.View at: Publisher Site | Google Scholar
H. Mittal, A. al Alili, P. P. Morajkar, and S. M. Alhassan, “Graphene oxide crosslinked hydrogel nanocomposites of xanthan gum for the adsorption of crystal violet dye,” Journal of Molecular Liquids, vol. 323, p. 115034, 2021.View at: Publisher Site | Google Scholar
M. M. Khan, S. F. Adil, and A. Al-Mayouf, “Metal oxides as photocatalysts,” Journal of Saudi Chemical Society, vol. 19, no. 5, pp. 462–464, 2015.View at: Publisher Site | Google Scholar
R. El-Salamony, “Advances in photo-catalytic materials for environmental applications,” Research & Reviews: Journal of Material Sciences, vol. 4, no. 2, pp. 26–50, 2016.View at: Google Scholar
I. K. Konstantinou and T. A. Albanis, “TiO2-assisted photocatalytic degradation of azo dyes in aqueous solution: kinetic and mechanistic investigations: a review,” Applied Catalysis B: Environmental, vol. 49, no. 1, pp. 1–14, 2004.View at: Publisher Site | Google Scholar
A. Ajmal, I. Majeed, R. N. Malik, H. Idriss, and M. A. Nadeem, “Principles and mechanisms of photocatalytic dye degradation on TiO2 based photocatalysts: a comparative overview,” RSC Advances, vol. 4, no. 70, pp. 37003–37026, 2014.View at: Publisher Site | Google Scholar
U. G. Akpan and B. H. Hameed, “Parameters affecting the photocatalytic degradation of dyes using TiO2-based photocatalysts: a review,” Journal of Hazardous Materials, vol. 170, no. 2-3, pp. 520–529, 2009.View at: Publisher Site | Google Scholar
L. Liu, H. Liu, Y. P. Zhao et al., “Directed synthesis of hierarchical nanostructured TiO2 catalysts and their morphology-dependent photocatalysis for phenol degradation,” Environmental Science & Technology, vol. 42, no. 7, pp. 2342–2348, 2008.View at: Publisher Site | Google Scholar
U. I. Gaya and A. H. Abdullah, “Heterogeneous photocatalytic degradation of organic contaminants over titanium dioxide: a review of fundamentals, progress and problems,” Journal of Photochemistry and Photobiology C: Photochemistry Reviews, vol. 9, no. 1, pp. 1–12, 2008.View at: Publisher Site | Google Scholar
J. Pal and T. Pal, “Faceted metal and metal oxide nanoparticles: design, fabrication and catalysis,” Nanoscale, vol. 7, no. 34, pp. 14159–14190, 2015.View at: Publisher Site | Google Scholar
Y. Liao, W. Que, Q. Jia, Y. He, J. Zhang, and P. Zhong, “Controllable synthesis of brookite/anatase/rutile TiO2 nanocomposites and single-crystalline rutile nanorods array,” Journal of Materials Chemistry, vol. 22, no. 16, pp. 7937–7944, 2012.View at: Publisher Site | Google Scholar
T. Luttrell, S. Halpegamage, J. Tao, A. Kramer, E. Sutter, and M. Batzill, “Why is anatase a better photocatalyst than rutile?-model studies on epitaxial TiO2 films,” Scientific Reports, vol. 4, no. 1, pp. 1–8, 2014.View at: Publisher Site | Google Scholar
T. Van Gerven, G. Mul, J. Moulijn, and A. Stankiewicz, “A review of intensification of photocatalytic processes,” Chemical Engineering and Processing: Process Intensification, vol. 46, no. 9, pp. 781–789, 2007.View at: Publisher Site | Google Scholar
S. W. Verbruggen, “TiO2 photocatalysis for the degradation of pollutants in gas phase: from morphological design to plasmonic enhancement,” Journal of Photochemistry and Photobiology C: Photochemistry Reviews, vol. 24, pp. 64–82, 2015.View at: Publisher Site | Google Scholar
V. Augugliaro, M. Bellardita, V. Loddo, G. Palmisano, L. Palmisano, and S. Yurdakal, “Overview on oxidation mechanisms of organic compounds by TiO2 in heterogeneous photocatalysis,” Journal of Photochemistry and Photobiology C: Photochemistry Reviews, vol. 13, no. 3, pp. 224–245, 2012.View at: Publisher Site | Google Scholar
H. Dong, G. Zeng, L. Tang et al., “An overview on limitations of TiO2-based particles for photocatalytic degradation of organic pollutants and the corresponding countermeasures,” Water Research, vol. 79, pp. 128–146, 2015.View at: Publisher Site | Google Scholar
I. Bannat, K. Wessels, T. Oekermann, J. Rathousky, D. Bahnemann, and M. Wark, “Improving the photocatalytic performance of mesoporous titania films by modification with gold nanostructures,” Chemistry of Materials, vol. 21, no. 8, pp. 1645–1653, 2009.View at: Publisher Site | Google Scholar
J. Zhang, Y. Wu, M. Xing, S. A. K. Leghari, and S. Sajjad, “Development of modified N doped TiO2 photocatalyst with metals, nonmetals and metal oxides,” Energy & Environmental Science, vol. 3, no. 6, pp. 715–726, 2010.View at: Publisher Site | Google Scholar
F. Dong, S. Guo, H. Wang, X. Li, and Z. Wu, “Enhancement of the visible light photocatalytic activity of C-doped TiO2 nanomaterials prepared by a green synthetic approach,” The Journal of Physical Chemistry C, vol. 115, no. 27, pp. 13285–13292, 2011.View at: Publisher Site | Google Scholar
Q. Li, Y. W. Li, P. Wu, R. Xie, and J. K. Shang, “Palladium oxide nanoparticles on nitrogen-doped titanium oxide: accelerated photocatalytic disinfection and post-illumination catalytic “memory”,” Advanced Materials, vol. 20, no. 19, pp. 3717–3723, 2008.View at: Publisher Site | Google Scholar
I. V. Lightcap, T. H. Kosel, and P. V. Kamat, “Anchoring semiconductor and metal nanoparticles on a two-dimensional catalyst mat. Storing and shuttling electrons with reduced graphene oxide,” Nano Letters, vol. 10, no. 2, pp. 577–583, 2010.View at: Publisher Site | Google Scholar
G. Williams, B. Seger, and P. V. Kamat, “TiO2-graphene nanocomposites. UV-assisted photocatalytic reduction of graphene oxide,” ACS Nano, vol. 2, no. 7, pp. 1487–1491, 2008.View at: Publisher Site | Google Scholar
O. Carp, C. L. Huisman, and A. Reller, “Photoinduced reactivity of titanium dioxide,” Progress in Solid State Chemistry, vol. 32, no. 1-2, pp. 33–177, 2004.View at: Publisher Site | Google Scholar
N. Nakayama and T. Hayashi, “Preparation and characterization of poly(l-lactic acid)/TiO2 nanoparticle nanocomposite films with high transparency and efficient photodegradability,” Polymer Degradation and Stability, vol. 92, no. 7, pp. 1255–1264, 2007.View at: Publisher Site | Google Scholar
T. A. Gad-Allah, S. Kato, S. Satokawa, and T. Kojima, “Role of core diameter and silica content in photocatalytic activity of TiO2/SiO2/Fe3O4 composite,” Solid State Sciences, vol. 9, no. 8, pp. 737–743, 2007.View at: Publisher Site | Google Scholar
Y. Tang, G. Zhang, C. Liu et al., “Magnetic TiO2-graphene composite as a high-performance and recyclable platform for efficient photocatalytic removal of herbicides from water,” Journal of Hazardous Materials, vol. 252-253, pp. 115–122, 2013.View at: Publisher Site | Google Scholar
S. Guggenheim and R. Martin, “Definition of clay and clay mineral: joint report of the AIPEA nomenclature and CMS nomenclature committees,” Clays and Clay Minerals, vol. 43, no. 2, pp. 255-256, 1995.View at: Publisher Site | Google Scholar
R. M. Zakaria, I. Hassan, M. Z. El-Abd, and Y. A. El-Tawil, “Lactic acid removal from wastewater by using different types of activated clay,” in Thirteenth international water technology conference (IWTC), Hurghada, 2009, Citeseer.View at: Google Scholar
G. Sheng, R. Shen, H. Dong, and Y. Li, “Colloidal diatomite, radionickel, and humic substance interaction: a combined batch, XPS, and EXAFS investigation,” Environmental Science and Pollution Research, vol. 20, no. 6, pp. 3708–3717, 2013.View at: Publisher Site | Google Scholar
A. Miller, Homogenized behavior from increasingly heterogeneous systems: uranium transport experiments at the intermediate scale, Colorado School of Mines, 2010.
A. W. Miller and Y. Wang, “Radionuclide interaction with clays in dilute and heavily compacted systems: a critical review,” Environmental Science & Technology, vol. 46, no. 4, pp. 1981–1994, 2012.View at: Publisher Site | Google Scholar
N. Parekh, J. M. Poskitt, B. A. Dodd, E. D. Potter, and A. Sanchez, “Soil microorganisms determine the sorption of radionuclides within organic soil systems,” Journal of Environmental Radioactivity, vol. 99, no. 5, pp. 841–852, 2008.View at: Publisher Site | Google Scholar
S. M. Rao and T. Thyagaraj, “Role of direction of salt migration on the swelling behaviour of compacted clays,” Applied Clay Science, vol. 38, no. 1-2, pp. 113–129, 2007.View at: Publisher Site | Google Scholar
G. Sheng, S. Yang, J. Sheng, J. Hu, X. Tan, and X. Wang, “Macroscopic and microscopic investigation of Ni (II) sequestration on diatomite by batch, XPS, and EXAFS techniques,” Environmental Science & Technology, vol. 45, no. 18, pp. 7718–7726, 2011.View at: Publisher Site | Google Scholar
S. Yang, J. Hu, C. Chen, D. Shao, and X. Wang, “Mutual effects of Pb (II) and humic acid adsorption on multiwalled carbon nanotubes/polyacrylamide composites from aqueous solutions,” Environmental Science & Technology, vol. 45, no. 8, pp. 3621–3627, 2011.View at: Publisher Site | Google Scholar
E. Manova, P. Aranda, M. Angeles Martín-Luengo, S. Letaïef, and E. Ruiz-Hitzky, “New titania-clay nanostructured porous materials,” Microporous and Mesoporous Materials, vol. 131, no. 1-3, pp. 252–260, 2010.View at: Publisher Site | Google Scholar
M. Tahir and N. S. Amin, “Photocatalytic reduction of carbon dioxide with water vapors over montmorillonite modified TiO2 nanocomposites,” Applied Catalysis B: Environmental, vol. 142-143, pp. 512–522, 2013.View at: Publisher Site | Google Scholar
H. Nishikiori, M. Furukawa, and T. Fujii, “Degradation of trichloroethylene using highly adsorptive allophane–TiO2 nanocomposite,” Applied Catalysis B: Environmental, vol. 102, no. 3-4, pp. 470–474, 2011.View at: Publisher Site | Google Scholar
R. Liu, Z. Ji, J. Wang, and J. Zhang, “Solvothermal synthesized Ag-decorated TiO2/sepiolite composite with enhanced UV–vis and visible light photocatalytic activity,” Microporous and Mesoporous Materials, vol. 266, pp. 268–275, 2018.View at: Publisher Site | Google Scholar
Z. Wang, Q. Xu, T. Meng, T. Ren, and D. Chen, “Preparation and characterization of CdS/TiO2–Mt composites with enhanced visible light photocatalytic activity,” Energy and Environment Focus, vol. 4, no. 2, pp. 149–156, 2015.View at: Publisher Site | Google Scholar
L. Yuan, D. Huang, W. Guo, Q. Yang, and J. Yu, “TiO2/montmorillonite nanocomposite for removal of organic pollutant,” Applied Clay Science, vol. 53, no. 2, pp. 272–278, 2011.View at: Publisher Site | Google Scholar
I. Fatimah, R. Nurillahi, I. Sahroni, and O. Muraza, “TiO2-pillared saponite and photosensitization using a ruthenium complex for photocatalytic enhancement of the photodegradation of bromophenol blue,” Applied Clay Science, vol. 183, article 105302, 2019.View at: Publisher Site | Google Scholar
V. Vinayagam and P. Thangaraju, “Equilibrium and kinetics of adsorption of cationic dyes by STISHOVITE clay-TiO2 nanocomposite,” International Journal of Modern Engineering Research, vol. 2, p. 3989, 2012.View at: Google Scholar
I. S. Al-Jobouri, S. A. Dhahir, and K. A. Al-Saade, “Adsorption study of Rhodamin B dye on Iraqi bentonite and modified bentonite by nanocompounds TIO2, ZnO, AL2O3 and sodium dodecyl sulfate,” American Journal of Environmental Sciences, vol. 9, no. 3, pp. 269–279, 2013.View at: Publisher Site | Google Scholar
Y. Lu, P. R. Chang, P. Zheng, and X. Ma, “Rectorite–TiO2–Fe3O4 composites: assembly, characterization, adsorption and photodegradation,” Chemical Engineering Journal, vol. 255, pp. 49–54, 2014.View at: Publisher Site | Google Scholar
C. Yang, Y. Zhu, J. Wang, Z. Li, X. Su, and C. Niu, “Hydrothermal synthesis of TiO2–WO3–bentonite composites: conventional versus ultrasonic pretreatments and their adsorption of methylene blue,” Applied Clay Science, vol. 105-106, pp. 243–251, 2015.View at: Publisher Site | Google Scholar
H. Zhao, F. Qiu, J. Yan, J. Wang, X. Li, and D. Yang, “Preparation of economical and environmentally friendly graphene/palygorskite/TiO2 composites and its application for the removal of methylene blue,” Applied Clay Science, vol. 121-122, pp. 137–145, 2016.View at: Publisher Site | Google Scholar
L. Laysandra, M. W. M. K. Sari, F. E. Soetaredjo et al., “Adsorption and photocatalytic performance of bentonite-titanium dioxide composites for methylene blue and rhodamine B decoloration,” Heliyon, vol. 3, no. 12, article e00488, 2017.View at: Publisher Site | Google Scholar
P. L. A. Guillaume, A. M. Chelaru, M. Visa, and O. Lassine, ““Titanium oxide-clay” as adsorbent and photocatalysts for wastewater treatment,” Journal of Membrane Science & Technology, vol. 8, no. 1, pp. 176–186, 2018.View at: Publisher Site | Google Scholar
E. Nyankson, B. Agyei-Tuffour, J. Adjasoo et al., “Synthesis and application of Fe-doped TiO2-halloysite nanotubes composite and their potential application in water treatment,” Advances in Materials Science and Engineering, vol. 2019, 15 pages, 2019.View at: Publisher Site | Google Scholar
Q. Wang, D. Gao, C. Gao et al., “Removal of a cationic dye by adsorption/photodegradation using electrospun PAN/O-MMT composite nanofibrous membranes coated with,” International Journal of Photoenergy, vol. 2012, 8 pages, 2012.View at: Publisher Site | Google Scholar
Y. Du and P. Zheng, “Adsorption and photodegradation of methylene blue on TiO2-halloysite adsorbents,” Korean Journal of Chemical Engineering, vol. 31, no. 11, pp. 2051–2056, 2014.View at: Publisher Site | Google Scholar
Y. Ngoh and M. Nawi, “Fabrication and properties of an immobilized P25TiO2-montmorillonite bilayer system for the synergistic photocatalytic–adsorption removal of methylene blue,” Materials Research Bulletin, vol. 76, pp. 8–21, 2016.View at: Publisher Site | Google Scholar
W. Hajjaji, S. Andrejkovičová, R. C. Pullar et al., “Effective removal of anionic and cationic dyes by kaolinite and TiO2/kaolinite composites,” Clay Minerals, vol. 51, no. 1, pp. 19–27, 2016.View at: Publisher Site | Google Scholar
L. Surya, P. V. P. Sheilatina, and N. S. Sepia, “Preparation and characterization of titania/bentonite composite application on the degradation of naphthol blue black dye,” Research Journal of Chemistry and Environment, vol. 22, no. II, pp. 48–53, 2018.View at: Google Scholar
T. Taher, A. Wulandari, R. Mohadi, and A. Lesbani, “TiO2/kaolin composite as low-cost adsorbent for procion red removal from aqueous solution: kinetics, equilibrium, and thermodynamic studies,” Bulletin of the Chemical Society of Ethiopia, vol. 33, no. 3, pp. 437–450, 2019.View at: Publisher Site | Google Scholar
Y. Zhang, H. Gan, and G. Zhang, “A novel mixed-phase TiO2/kaolinite composites and their photocatalytic activity for degradation of organic contaminants,” Chemical Engineering Journal, vol. 172, no. 2-3, pp. 936–943, 2011.View at: Publisher Site | Google Scholar
M. Trujillo, D. Hirales, M. E. Rincón, J. F. Hinojosa, G. L. Leyva, and F. F. Castillón, “TiO2/clinoptilolite composites for photocatalytic degradation of anionic and cationic contaminants,” Journal of Materials Science, vol. 48, no. 19, pp. 6778–6785, 2013.View at: Publisher Site | Google Scholar
A. Rapsomanikis, D. Papoulis, D. Panagiotaras, E. Kaplani, and E. Stathatos, “Nanocrystalline TiO2 and halloysite clay mineral composite films prepared by sol-gel method: synergistic effect and the case of silver modification to the photocatalytic degradation of basic blue-41 azo dye in water,” Global NEST Journal, vol. 16, no. 3, pp. 485–498, 2019.View at: Google Scholar
Y. Yang, R. Liu, G. Zhang, L. Gao, and W. Zhang, “Preparation and photocatalytic properties of visible light driven Ag–AgCl–TiO2/palygorskite composite,” Journal of Alloys and Compounds, vol. 657, pp. 801–808, 2016.View at: Publisher Site | Google Scholar
O. A. Zelekew, D. H. Kuo, J. M. Yassin, K. E. Ahmed, and H. Abdullah, “Synthesis of efficient silica supported TiO2/Ag2O heterostructured catalyst with enhanced photocatalytic performance,” Applied Surface Science, vol. 410, pp. 454–463, 2017.View at: Publisher Site | Google Scholar
A. Mishra, A. Mehta, S. Kainth, and S. Basu, “Effect of g-C3N4 loading on TiO2/bentonite nanocomposites for efficient heterogeneous photocatalytic degradation of industrial dye under visible light,” Journal of Alloys and Compounds, vol. 764, pp. 406–415, 2018.View at: Publisher Site | Google Scholar
V. Wongso, C. J. Chen, A. Razzaq, N. A. Kamal, and N. S. Sambudi, “Hybrid kaolin/TiO2 composite: effect of urea addition towards an efficient photocatalyst for dye abatement under visible light irradiation,” Applied Clay Science, vol. 180, p. 105158, 2019.View at: Publisher Site | Google Scholar
I. Labib, H. Boutoumi, and H. Khalaf, “Synergistic effect of microwave calcination and sonophotocatalytic activity of TiO2-montmorillonite on the degradation of direct yellow 106 and disperse violet 1,” Bulletin of Chemical Reaction Engineering & Catalysis, vol. 15, no. 2, pp. 304–318, 2020.View at: Publisher Site | Google Scholar
Y. Zhang, D. Wang, and G. Zhang, “Photocatalytic degradation of organic contaminants by TiO2/sepiolite composites prepared at low temperature,” Chemical Engineering Journal, vol. 173, no. 1, pp. 1–10, 2011.View at: Publisher Site | Google Scholar
K. M. Kutláková, J. Tokarský, P. Kovář et al., “Preparation and characterization of photoactive composite kaolinite/TiO2,” Journal of Hazardous Materials, vol. 188, no. 1-3, pp. 212–220, 2011.View at: Publisher Site | Google Scholar
Y. Zhang, L. Deng, G. Zhang, and H. Gan, “Facile synthesis and photocatalytic property of bicrystalline TiO2/rectorite composites,” Colloids and Surfaces A: Physicochemical and Engineering Aspects, vol. 384, no. 1-3, pp. 137–144, 2011.View at: Publisher Site | Google Scholar
X. Gu, J. L. Jiang, and D. Li, “Synthesis and characterization of attapulgite clay coated Ag/AgBr/TiO2 visible light photocatalyst,” Advanced Materials Research, vol. 178, pp. 285–290, 2010.View at: Publisher Site | Google Scholar
Y. Zhang, Y. Guo, G. Zhang, and Y. Gao, “Stable TiO2/rectorite: preparation, characterization and photocatalytic activity,” Applied Clay Science, vol. 51, no. 3, pp. 335–340, 2011.View at: Publisher Site | Google Scholar
Q. Wang, X. Wang, X. Li, Y. Cai, and Q. Wei, “Surface modification of PMMA/O-MMT composite microfibers by TiO2 coating,” Applied Surface Science, vol. 258, no. 1, pp. 98–102, 2011.View at: Publisher Site | Google Scholar
K. Chen, J. Li, W. Wang, Y. Zhang, X. Wang, and H. Su, “The preparation of vanadium-doped TiO2–montmorillonite nanocomposites and the photodegradation of sulforhodamine B under visible light irradiation,” Applied Surface Science, vol. 257, no. 16, pp. 7276–7285, 2011.View at: Publisher Site | Google Scholar
Y. Lin, P. Pi, Z. Yang, and L. Wang, “Synthesis and photocatalytic property of the ZrO2/TiO2 pillared laponite,” Journal of Wuhan University of Technology-Materials Science Edition, vol. 26, no. 5, pp. 852–856, 2011.View at: Publisher Site | Google Scholar
J. Xia, Y. Tang, Z. Zhang, and Y. Wang, “RTB photocatalytic degradation for neutral red,” Environmental Science & Technology, vol. 34, no. 2, pp. 59–63, 2011.View at: Google Scholar
S. H. Mao, R. P. Wang, Y. Wang et al., Photocatalytic performance of TiO_2/bentonite pillared composite prepared with modified bentonite, Applied Chemical Industry, 2011.
D. Chen, Q. Zhu, F. Zhou, X. Deng, and F. Li, “Synthesis and photocatalytic performances of the TiO2 pillared montmorillonite,” Journal of Hazardous Materials, vol. 235-236, pp. 186–193, 2012.View at: Publisher Site | Google Scholar
B. X. Zhao, L. P. Dang, X. L. Zhang, N. Yang, and Y. Y. Sun, “Preparation of TiO2-pillared montmorillonite as photocatalyst and photocatalytic degradation of methyl orange,” Applied Mechanics and Materials, vol. 190-191, pp. 534–538, 2012.View at: Publisher Site | Google Scholar
W. Hajjaji, S. O. Ganiyu, D. M. Tobaldi et al., “Natural Portuguese clayey materials and derived TiO2-containing composites used for decolouring methylene blue (MB) and orange II (OII) solutions,” Applied Clay Science, vol. 83-84, pp. 91–98, 2013.View at: Publisher Site | Google Scholar
K. Sandhya, S. Haridas, and S. Sugunan, “Visible light induced photocatalytic activity of polyaniline modified TiO2 and clay-TiO2 composites,” Bulletin of Chemical Reaction Engineering & Catalysis, vol. 8, no. 2, pp. 145–153, 2013.View at: Publisher Site | Google Scholar
C. Li, J. Wang, S. Feng, Z. Yang, and S. Ding, “Low-temperature synthesis of heterogeneous crystalline TiO2–halloysite nanotubes and their visible light photocatalytic activity,” Journal of Materials Chemistry A, vol. 1, no. 27, pp. 8045–8054, 2013.View at: Publisher Site | Google Scholar
L.-K. Meng, C.-Y. Cao, and K. Tang, “Study on disposal of textile dyes in aqueous solution by TiO2Pillared bentonite,” Separation Science and Technology, vol. 48, no. 15, pp. 2302–2306, 2013.View at: Publisher Site | Google Scholar
N. Khalfaoui-Boutoumi, H. Boutoumi, H. Khalaf, and B. David, “Synthesis and characterization of TiO2–montmorillonite/polythiophene-SDS nanocomposites: application in the sonophotocatalytic degradation of rhodamine 6G,” Applied Clay Science, vol. 80-81, pp. 56–62, 2013.View at: Publisher Site | Google Scholar
L. Bouna, B. Rhouta, and F. Maury, “Physicochemical study of photocatalytic activity of TiO2 supported palygorskite clay mineral,” International Journal of Photoenergy, vol. 2013, 6 pages, 2013.View at: Publisher Site | Google Scholar
H. B. Hadjltaief, M. E. Galvez, M. B. Zina, and P. Da Costa, “TiO2/clay as a heterogeneous catalyst in photocatalytic/photochemical oxidation of anionic reactive blue 19,” Arabian Journal of Chemistry, vol. 12, no. 7, pp. 1454–1462, 2019.View at: Publisher Site | Google Scholar
R. Djellabi, M. F. Ghorab, G. Cerrato et al., “Photoactive TiO2–montmorillonite composite for degradation of organic dyes in water,” Journal of Photochemistry and Photobiology A: Chemistry, vol. 295, pp. 57–63, 2014.View at: Publisher Site | Google Scholar
J. Zhang, L. Zhang, Lv et al., “Exceptional visible-light-induced photocatalytic activity of attapulgite–BiOBr–TiO2 nanocomposites,” Applied Clay Science, vol. 90, pp. 135–140, 2014.View at: Publisher Site | Google Scholar
L. Bouna, B. Rhouta, F. Maury, A. Jada, F. Senocq, and M. . C. Lafont, “Photocatalytic activity of TiO2/stevensite nanocomposites for the removal of orange G from aqueous solutions,” Clay Minerals, vol. 49, no. 3, pp. 417–428, 2014.View at: Publisher Site | Google Scholar
D. Zhang, “Photocatalytic degradation of organic compounds by Au-TiO2/sepiolite composites as the highly efficient catalysts,” Russian Journal of Physical Chemistry A, vol. 88, no. 12, pp. 2252–2259, 2014.View at: Publisher Site | Google Scholar
D. Chen, Y. du, H. Zhu, and Y. Deng, “Synthesis and characterization of a microfibrous TiO2–CdS/palygorskite nanostructured material with enhanced visible-light photocatalytic activity,” Applied Clay Science, vol. 87, pp. 285–291, 2014.View at: Publisher Site | Google Scholar
Y. Du, D. Tang, G. Zhang, and X. Wu, “Facile synthesis of Ag2O-TiO2/sepiolite composites with enhanced visible-light photocatalytic properties,” Chinese Journal of Catalysis, vol. 36, no. 12, pp. 2219–2228, 2015.View at: Publisher Site | Google Scholar
W. Chen, H. Xiao, H. Xu, T. Ding, and Y. Gu, “Photodegradation of methylene blue by TiO2-Fe3O4-bentonite magnetic nanocomposite,” International Journal of Photoenergy, vol. 2015, 7 pages, 2015.View at: Publisher Site | Google Scholar
P. Yao, S. Zhong, and Z. Shen, “TiO2/halloysite composites codoped with carbon and nitrogen from melamine and their enhanced solar-light-driven photocatalytic performance,” International Journal of Photoenergy, vol. 2015, 8 pages, 2015.View at: Publisher Site | Google Scholar
B. Han, Q. Dong, J. Chen, W. Feng, S. Liu, and H. L. Wang, “Photocatalytic degradation of methyl orange over Y3+ doped TiO2 pillared montmorillonite,” Journal of Advanced Oxidation Technologies, vol. 18, no. 1, pp. 98–104, 2015.View at: Publisher Site | Google Scholar
P. Zheng, Y. du, P. R. Chang, and X. Ma, “Amylose–halloysite–TiO2 composites: preparation, characterization and photodegradation,” Applied Surface Science, vol. 329, pp. 256–261, 2015.View at: Publisher Site | Google Scholar
F. Zhou, C. Yan, T. Liang, Q. Sun, and H. Wang, “Photocatalytic degradation of orange G using sepiolite-TiO2 nanocomposites: optimization of physicochemical parameters and kinetics studies,” Chemical Engineering Science, vol. 183, pp. 231–239, 2018.View at: Publisher Site | Google Scholar
A. Pohan, H. Goure-Doubi, A. Kouyate, M. Nasir, M. Visa, and L. Ouattara, “Hydrothermal sol-gel TiO2 nanoparticles fixed to clay and its photocatalytic application for the degradation of methyl orange,” Mediterranean Journal of Chemistry, vol. 9, no. 2, pp. 125–132, 2019.View at: Publisher Site | Google Scholar
W. V. de Oliveira, A. Í. S. Morais, L. M. C. Honorio et al., “TiO2 immobilized on fibrous clay as strategies to photocatalytic activity,” Materials Research, vol. 23, no. 1, 2020.View at: Publisher Site | Google Scholar